#------------------------------------------------------------------------------
#$Date: 2016-03-24 14:36:54 +0200 (Thu, 24 Mar 2016) $
#$Revision: 179669 $
#$URL: svn://www.crystallography.net/cod/cif/4/51/22/4512295.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4512295
loop_
_publ_author_name
'Zhao, Jun-Wei'
'Cao, Jing'
'Li, Yan-Zhou'
'Zhang, Jing'
'Chen, Li-Juan'
_publ_section_title
;
 First Tungstoantimonate-Based Transition-Metal--Lanthanide Heterometallic
 Hybrids Functionalized by Amino Acid Ligands
;
_journal_issue                   12
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              6217
_journal_paper_doi               10.1021/cg5007988
_journal_volume                  14
_journal_year                    2014
_chemical_formula_sum            'C8 H110 Eu2 Fe4 N2 O118 Sb2 W18'
_chemical_formula_weight         6203.10
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                106.9480(10)
_cell_angle_beta                 99.9240(10)
_cell_angle_gamma                96.9080(10)
_cell_formula_units_Z            1
_cell_length_a                   12.6012(6)
_cell_length_b                   13.5607(6)
_cell_length_c                   16.2390(7)
_cell_measurement_reflns_used    8916
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      25.00
_cell_measurement_theta_min      1.90
_cell_volume                     2571.5(2)
_computing_cell_refinement       'Bruker XSCANS'
_computing_data_collection       'Bruker XSCANS'
_computing_data_reduction        'Bruker SHELXTL'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_detector_area_resol_mean none
_diffrn_measured_fraction_theta_full 0.985
_diffrn_measured_fraction_theta_max 0.985
_diffrn_measurement_device_type  'Bruker P4'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0293
_diffrn_reflns_av_sigmaI/netI    0.0533
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            13203
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.90
_diffrn_standards_decay_%        none
_diffrn_standards_interval_count none
_diffrn_standards_interval_time  none
_diffrn_standards_number         none
_exptl_absorpt_coefficient_mu    22.432
_exptl_absorpt_correction_T_max  0.1238
_exptl_absorpt_correction_T_min  0.0403
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            'green yellow'
_exptl_crystal_density_diffrn    4.006
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'cubic block'
_exptl_crystal_F_000             2780
_exptl_crystal_size_max          0.40
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.16
_refine_diff_density_max         3.247
_refine_diff_density_min         -2.654
_refine_diff_density_rms         0.331
_refine_ls_extinction_coef       0.00032(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.063
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     639
_refine_ls_number_reflns         8916
_refine_ls_number_restraints     14
_refine_ls_restrained_S_all      1.064
_refine_ls_R_factor_all          0.0435
_refine_ls_R_factor_gt           0.0393
_refine_ls_shift/su_max          0.004
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0317P)²+58.7474P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0927
_refine_ls_wR_factor_ref         0.0948
_reflns_number_gt                8196
_reflns_number_total             8916
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg5007988_si_002.cif
_cod_data_source_block           4
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to
/home/saulius/struct/COD-crude-data--automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2935 2014-11-11 08:27:57Z andrius 

 Adding full bibliography for 4512292--4512298.cif.
;
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               4512295
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Sb1 Sb 0.35725(6) 0.35989(6) 0.34601(5) 0.00874(17) Uani 1 1 d .
W1 W 0.35688(4) 0.61547(4) 0.47126(3) 0.01007(12) Uani 1 1 d .
W2 W 0.09777(4) 0.48673(4) 0.37931(3) 0.01220(12) Uani 1 1 d .
W3 W 0.24879(4) 0.57439(4) 0.25582(3) 0.01274(12) Uani 1 1 d .
W4 W 0.46869(4) 0.43887(4) 0.17937(3) 0.01303(12) Uani 1 1 d .
W5 W 0.21482(4) 0.31105(4) 0.09634(3) 0.01309(12) Uani 1 1 d .
W6 W 0.04529(4) 0.21488(4) 0.23231(3) 0.01258(12) Uani 1 1 d .
W7 W 0.15166(4) 0.25456(4) 0.44322(3) 0.01375(13) Uani 1 1 d .
W8 W 0.24615(4) 0.08976(4) 0.28994(3) 0.01428(13) Uani 1 1 d .
W9 W 0.41464(4) 0.18385(4) 0.15311(3) 0.01520(13) Uani 1 1 d .
Fe1 Fe 0.37871(13) 0.42927(12) 0.60198(11) 0.0115(4) Uani 1 1 d .
O1W O 0.2414(7) 0.4523(7) 0.6530(7) 0.025(2) Uani 1 1 d .
O2W O 0.4085(8) 0.3187(7) 0.6630(7) 0.026(2) Uani 1 1 d .
O5W O 0.0197(15) 0.3788(14) -0.1206(13) 0.092 Uiso 1 1 d .
O6W O 0.2742(11) 0.3786(10) -0.0960(8) 0.054(4) Uani 1 1 d .
O7W O 0.0830(18) 0.3476(17) -0.2652(15) 0.116(7) Uiso 1 1 d .
O8W O -0.0574(14) 0.1819(14) -0.2795(12) 0.084 Uiso 1 1 d .
O9W O 0.2422(13) 0.2245(14) -0.2697(10) 0.075(5) Uani 1 1 d .
O10W O 0.081(2) 0.0593(19) -0.2840(17) 0.130(8) Uiso 1 1 d .
O11W O 0.0114(18) 0.1047(15) -0.1257(13) 0.106(6) Uani 1 1 d U
O12W O 0.2553(14) 0.1472(12) -0.1188(11) 0.086(6) Uani 1 1 d .
O13W O 0.207(3) 0.019(3) 0.580(2) 0.089(11) Uani 0.50 1 d P
O14W O 0.354(2) 0.8800(11) 0.3991(11) 0.116(9) Uani 1 1 d .
O15W O -0.079(3) 0.468(3) -0.007(3) 0.098(12) Uani 0.50 1 d P
O16W O -0.1349(14) 0.2011(15) -0.0097(10) 0.085(5) Uani 1 1 d .
O17W O 0.1189(14) 0.0034(11) 0.0056(11) 0.083(5) Uani 1 1 d .
O18W O -0.0953(13) 0.3957(12) 0.1315(11) 0.074(5) Uani 1 1 d .
O19W O 0.2557(12) 0.6473(12) 0.7704(11) 0.075(5) Uani 1 1 d .
O20W O -0.1197(15) 0.1995(17) 0.5566(14) 0.103(6) Uani 1 1 d .
O21W O 0.1648(8) 0.7130(8) 0.6314(7) 0.035(3) Uani 1 1 d .
O23W O 0.303(2) 0.945(2) 0.8575(19) 0.145(9) Uiso 1 1 d .
O22W O 0.680(3) 0.132(3) 0.079(3) 0.097(11) Uiso 0.50 1 d P
O24W O 0.386(2) 1.0458(18) 0.8176(17) 0.053(7) Uani 0.50 1 d P
O25W O 0.3787(13) 0.1334(10) 0.5420(9) 0.067(5) Uani 1 1 d .
O1 O 0.4814(7) 0.5909(7) 0.4392(6) 0.0191(19) Uani 1 1 d .
O2 O 0.2748(6) 0.4775(6) 0.3540(5) 0.0104(17) Uani 1 1 d U
O3 O 0.3558(7) 0.5312(7) 0.5381(6) 0.019(2) Uani 1 1 d .
O4 O 0.3947(7) 0.7413(6) 0.5513(5) 0.0144(18) Uani 1 1 d .
O5 O 0.3130(11) 0.6708(12) 0.3687(10) 0.013(3) Uiso 0.80 1 d P
O5' O 0.332(5) 0.666(5) 0.361(4) 0.010 Uiso 0.20 1 d P
O6 O 0.1908(12) 0.6056(9) 0.4647(10) 0.011 Uiso 0.80 1 d P
O6' O 0.199(5) 0.585(4) 0.464(4) 0.010 Uiso 0.20 1 d P
O7 O -0.0260(7) 0.5167(7) 0.3979(6) 0.022(2) Uani 1 1 d .
O8 O 0.1232(7) 0.3938(6) 0.4434(5) 0.0146(18) Uani 1 1 d .
O9 O 0.0512(6) 0.3616(6) 0.2752(6) 0.0141(18) Uani 1 1 d .
O10 O 0.1147(12) 0.5618(10) 0.2918(10) 0.010 Uiso 0.80 1 d P
O10' O 0.109(5) 0.545(4) 0.299(4) 0.010 Uiso 0.20 1 d P
O11 O 0.2225(8) 0.6612(7) 0.1985(6) 0.024(2) Uani 1 1 d .
O12 O 0.1870(7) 0.4376(6) 0.1648(5) 0.0155(18) Uani 1 1 d .
O13 O 0.3845(7) 0.5462(6) 0.2294(6) 0.0159(18) Uiso 1 1 d .
O14 O 0.3453(7) 0.3300(6) 0.2163(5) 0.0127(17) Uani 1 1 d .
O15 O 0.5574(8) 0.5092(8) 0.1393(7) 0.030(2) Uani 1 1 d .
O16 O 0.5015(7) 0.2998(7) 0.1346(6) 0.0171(19) Uani 1 1 d .
O17 O 0.5437(7) 0.4590(6) 0.2916(5) 0.0137(18) Uani 1 1 d .
O18 O 0.3418(7) 0.3938(7) 0.0809(6) 0.0161(18) Uani 1 1 d .
O19 O 0.1360(7) 0.2901(7) -0.0089(6) 0.019(2) Uani 1 1 d .
O20 O 0.2905(7) 0.1959(7) 0.0662(6) 0.0179(19) Uani 1 1 d .
O21 O 0.1178(7) 0.2354(6) 0.1421(6) 0.0157(18) Uani 1 1 d .
O22 O -0.0864(7) 0.1701(7) 0.1725(6) 0.020(2) Uani 1 1 d .
O23 O 0.2195(6) 0.2553(6) 0.3204(5) 0.0112(17) Uani 1 1 d .
O24 O 0.0975(6) 0.0854(6) 0.2211(6) 0.0160(19) Uani 1 1 d .
O25 O 0.0218(7) 0.2119(7) 0.3443(6) 0.0168(19) Uani 1 1 d .
O26 O 0.0891(8) 0.2384(7) 0.5259(6) 0.024(2) Uani 1 1 d .
O27 O 0.1817(7) 0.1170(6) 0.3949(6) 0.0154(18) Uani 1 1 d .
O28 O 0.2913(7) 0.3153(6) 0.5012(6) 0.0168(19) Uani 1 1 d .
O29 O 0.2346(8) -0.0456(7) 0.2673(6) 0.022(2) Uani 1 1 d .
O30 O 0.3010(7) 0.1082(7) 0.1929(6) 0.0173(19) Uani 1 1 d .
O31 O 0.3813(7) 0.1415(6) 0.3617(6) 0.0178(19) Uani 1 1 d .
O32 O 0.4573(7) 0.0798(7) 0.0843(6) 0.023(2) Uani 1 1 d .
O33 O 0.5038(7) 0.2086(7) 0.2620(6) 0.0171(19) Uani 1 1 d .
Eu1 Eu 0.11604(6) 0.23728(6) -0.17057(5) 0.02582(18) Uani 1 1 d .
Fe2 Fe 0.53272(14) 0.13397(13) 0.34590(12) 0.0151(4) Uani 1 1 d .
O3W O 0.6864(8) 0.1178(8) 0.3240(7) 0.032(2) Uani 1 1 d .
O4W O 0.5515(9) 0.0461(8) 0.4307(7) 0.036(3) Uani 1 1 d .
O34 O 0.4794(8) -0.0066(7) 0.2493(6) 0.025(2) Uani 1 1 d .
O35 O 0.5731(15) -0.1256(14) 0.2655(13) 0.088 Uiso 1 1 d .
H35A H 0.5901 -0.0923 0.3182 0.131 Uiso 1 1 calc R
O36 O 0.5175(14) -0.2138(14) 0.0550(12) 0.083 Uiso 1 1 d .
H36A H 0.5549 -0.1569 0.0853 0.125 Uiso 1 1 calc R
N1 N 0.3390(16) -0.1194(16) 0.1083(15) 0.084(6) Uiso 1 1 d D
H1A H 0.3216 -0.1364 0.0517 0.100 Uiso 1 1 calc R
H1B H 0.3128 -0.0699 0.1403 0.100 Uiso 1 1 calc R
C1 C 0.494(2) -0.089(2) 0.2265(19) 0.081 Uiso 1 1 d .
C2 C 0.413(2) -0.1750(19) 0.1501(17) 0.082 Uiso 1 1 d D
H2A H 0.3670 -0.2078 0.1810 0.098 Uiso 1 1 calc R
C3 C 0.465(2) -0.2590(17) 0.108(2) 0.091(9) Uani 1 1 d U
H3A H 0.5133 -0.2838 0.1489 0.110 Uiso 1 1 calc R
C4 C 0.377(3) -0.349(3) 0.033(2) 0.146(17) Uani 1 1 d U
H4A H 0.4135 -0.4010 0.0011 0.219 Uiso 1 1 calc R
H4D H 0.3380 -0.3191 -0.0075 0.219 Uiso 1 1 calc R
H4B H 0.3258 -0.3815 0.0589 0.219 Uiso 1 1 calc R
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Eu Eu -0.1578 3.6682 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O2 Sb1 O14 92.4(3) . .
O2 Sb1 O23 92.1(3) . .
O14 Sb1 O23 89.4(3) . .
O4 W1 O1 103.3(4) . .
O4 W1 O3 102.2(4) . .
O1 W1 O3 96.4(4) . .
O4 W1 O6' 101.6(15) . .
O1 W1 O6' 154.9(15) . .
O3 W1 O6' 80.8(15) . .
O4 W1 O5 94.3(5) . .
O1 W1 O5 91.0(4) . .
O3 W1 O5 159.8(5) . .
O6' W1 O5 84.5(17) . .
O4 W1 O6 95.4(4) . .
O1 W1 O6 159.6(5) . .
O3 W1 O6 87.3(5) . .
O6' W1 O6 8.2(14) . .
O5 W1 O6 79.5(5) . .
O4 W1 O5' 96.8(17) . .
O1 W1 O5' 82.9(17) . .
O3 W1 O5' 160.6(17) . .
O6' W1 O5' 92(2) . .
O5 W1 O5' 8.1(18) . .
O6 W1 O5' 87.0(17) . .
O4 W1 O2 164.3(3) . .
O1 W1 O2 86.3(3) . .
O3 W1 O2 88.8(3) . .
O6' W1 O2 68.8(16) . .
O5 W1 O2 72.9(5) . .
O6 W1 O2 73.7(4) . .
O5' W1 O2 71.8(17) . .
O7 W2 O10' 98(2) . .
O7 W2 O6' 105.4(16) . .
O10' W2 O6' 95(3) . .
O7 W2 O8 102.6(4) . .
O10' W2 O8 157(2) . .
O6' W2 O8 88.3(16) . .
O7 W2 O6 99.0(5) . .
O10' W2 O6 90(2) . .
O6' W2 O6 9.0(15) . .
O8 W2 O6 95.9(5) . .
O7 W2 O9 101.2(4) . .
O10' W2 O9 81.1(19) . .
O6' W2 O9 153.4(16) . .
O8 W2 O9 85.9(4) . .
O6 W2 O9 158.9(5) . .
O7 W2 O10 98.1(5) . .
O10' W2 O10 3(2) . .
O6' W2 O10 91.8(19) . .
O8 W2 O10 158.5(5) . .
O6 W2 O10 86.5(6) . .
O9 W2 O10 84.4(5) . .
O7 W2 O2 169.5(4) . .
O10' W2 O2 74(2) . .
O6' W2 O2 68.6(17) . .
O8 W2 O2 86.1(3) . .
O6 W2 O2 74.0(5) . .
O9 W2 O2 85.1(3) . .
O10 W2 O2 74.0(5) . .
O11 W3 O5' 100.3(19) . .
O11 W3 O10 97.7(5) . .
O5' W3 O10 97(2) . .
O11 W3 O5 99.5(6) . .
O5' W3 O5 9(2) . .
O10 W3 O5 88.6(6) . .
O11 W3 O13 100.2(4) . .
O5' W3 O13 85.1(19) . .
O10 W3 O13 161.2(4) . .
O5 W3 O13 94.0(4) . .
O11 W3 O12 102.2(4) . .
O5' W3 O12 156.6(19) . .
O10 W3 O12 85.9(5) . .
O5 W3 O12 158.2(5) . .
O13 W3 O12 84.8(4) . .
O11 W3 O10' 104.8(15) . .
O5' W3 O10' 97(3) . .
O10 W3 O10' 7.3(16) . .
O5 W3 O10' 89.1(18) . .
O13 W3 O10' 153.9(14) . .
O12 W3 O10' 82.8(17) . .
O11 W3 O2 169.9(4) . .
O5' W3 O2 73.0(19) . .
O10 W3 O2 76.0(4) . .
O5 W3 O2 72.8(5) . .
O13 W3 O2 87.0(3) . .
O12 W3 O2 85.4(3) . .
O10' W3 O2 69.2(15) . .
O15 W4 O17 103.2(4) . .
O15 W4 O16 100.9(4) . .
O17 W4 O16 93.3(4) . .
O15 W4 O18 100.5(4) . .
O17 W4 O18 156.0(4) . .
O16 W4 O18 86.5(4) . .
O15 W4 O13 100.7(4) . .
O17 W4 O13 88.3(4) . .
O16 W4 O13 157.5(4) . .
O18 W4 O13 83.1(4) . .
O15 W4 O14 173.0(4) . .
O17 W4 O14 82.2(3) . .
O16 W4 O14 74.2(3) . .
O18 W4 O14 74.6(3) . .
O13 W4 O14 83.7(3) . .
O19 W5 O12 104.5(4) . .
O19 W5 O21 100.7(4) . .
O12 W5 O21 90.9(4) . .
O19 W5 O20 97.6(4) . .
O12 W5 O20 157.1(4) . .
O21 W5 O20 91.2(4) . .
O19 W5 O18 95.5(4) . .
O12 W5 O18 86.2(4) . .
O21 W5 O18 163.8(4) . .
O20 W5 O18 85.5(4) . .
O19 W5 O14 167.6(4) . .
O12 W5 O14 83.9(3) . .
O21 W5 O14 88.1(3) . .
O20 W5 O14 73.3(3) . .
O18 W5 O14 75.7(3) . .
O22 W6 O9 102.6(4) . .
O22 W6 O25 98.8(4) . .
O9 W6 O25 86.8(4) . .
O22 W6 O24 100.9(4) . .
O9 W6 O24 156.3(3) . .
O25 W6 O24 86.9(4) . .
O22 W6 O21 100.3(4) . .
O9 W6 O21 88.7(4) . .
O25 W6 O21 160.9(3) . .
O24 W6 O21 89.9(4) . .
O22 W6 O23 171.8(4) . .
O9 W6 O23 83.5(3) . .
O25 W6 O23 75.9(3) . .
O24 W6 O23 72.8(3) . .
O21 W6 O23 85.1(3) . .
O26 W7 O28 103.3(4) . .
O26 W7 O27 100.9(4) . .
O28 W7 O27 96.2(4) . .
O26 W7 O8 100.5(4) . .
O28 W7 O8 88.3(4) . .
O27 W7 O8 156.5(4) . .
O26 W7 O25 99.3(4) . .
O28 W7 O25 156.3(4) . .
O27 W7 O25 86.1(4) . .
O8 W7 O25 80.8(3) . .
O26 W7 O23 172.1(4) . .
O28 W7 O23 83.3(3) . .
O27 W7 O23 73.9(3) . .
O8 W7 O23 83.8(3) . .
O25 W7 O23 74.7(3) . .
O29 W8 O31 103.5(4) . .
O29 W8 O30 101.1(4) . .
O31 W8 O30 90.5(4) . .
O29 W8 O27 96.9(4) . .
O31 W8 O27 89.3(4) . .
O30 W8 O27 161.5(3) . .
O29 W8 O24 96.2(4) . .
O31 W8 O24 160.3(4) . .
O30 W8 O24 87.1(4) . .
O27 W8 O24 86.9(4) . .
O29 W8 O23 166.5(4) . .
O31 W8 O23 87.1(3) . .
O30 W8 O23 87.1(3) . .
O27 W8 O23 74.5(3) . .
O24 W8 O23 73.3(3) . .
O32 W9 O33 104.3(4) . .
O32 W9 O16 100.0(4) . .
O33 W9 O16 91.4(4) . .
O32 W9 O30 100.5(4) . .
O33 W9 O30 87.4(4) . .
O16 W9 O30 159.0(4) . .
O32 W9 O20 97.9(4) . .
O33 W9 O20 157.5(4) . .
O16 W9 O20 88.7(4) . .
O30 W9 O20 84.6(4) . .
O32 W9 O14 167.4(4) . .
O33 W9 O14 87.1(3) . .
O16 W9 O14 74.1(3) . .
O30 W9 O14 85.0(3) . .
O20 W9 O14 71.2(3) . .
O17 Fe1 O28 175.0(4) 2_666 .
O17 Fe1 O3 91.0(4) 2_666 .
O28 Fe1 O3 91.2(4) . .
O17 Fe1 O1 91.7(4) 2_666 2_666
O28 Fe1 O1 92.8(4) . 2_666
O3 Fe1 O1 90.4(4) . 2_666
O17 Fe1 O2W 90.6(4) 2_666 .
O28 Fe1 O2W 87.5(4) . .
O3 Fe1 O2W 176.3(4) . .
O1 Fe1 O2W 86.3(4) 2_666 .
O17 Fe1 O1W 85.1(4) 2_666 .
O28 Fe1 O1W 90.3(4) . .
O3 Fe1 O1W 91.9(4) . .
O1 Fe1 O1W 176.0(4) 2_666 .
O2W Fe1 O1W 91.5(4) . .
W1 O1 Fe1 175.8(5) . 2_666
Sb1 O2 W1 110.5(4) . .
Sb1 O2 W2 129.0(4) . .
W1 O2 W2 94.8(3) . .
Sb1 O2 W3 127.9(4) . .
W1 O2 W3 95.2(3) . .
W2 O2 W3 90.9(3) . .
W1 O3 Fe1 168.9(6) . .
W1 O4 Fe2 165.2(5) . 2_666
W3 O5 W1 119.0(8) . .
W3 O5' W1 119(3) . .
W2 O6 W1 116.9(6) . .
W2 O6' W1 128(3) . .
W2 O8 W7 148.1(5) . .
W6 O9 W2 144.7(5) . .
W3 O10 W2 119.1(7) . .
W2 O10' W3 125(3) . .
W5 O12 W3 146.7(5) . .
W3 O13 W4 146.7(5) . .
Sb1 O14 W5 137.8(4) . .
Sb1 O14 W4 114.7(3) . .
W5 O14 W4 93.1(3) . .
Sb1 O14 W9 112.9(4) . .
W5 O14 W9 95.5(3) . .
W4 O14 W9 93.0(3) . .
W9 O16 W4 118.7(4) . .
W4 O17 Fe1 140.8(5) . 2_666
W5 O18 W4 116.0(4) . .
W5 O19 Eu1 150.3(5) . .
W5 O20 W9 119.9(4) . .
W5 O21 W6 154.1(5) . .
Sb1 O23 W8 113.7(4) . .
Sb1 O23 W7 114.0(4) . .
W8 O23 W7 94.1(3) . .
Sb1 O23 W6 138.2(4) . .
W8 O23 W6 95.5(3) . .
W7 O23 W6 91.8(3) . .
W6 O24 W8 118.5(4) . .
W6 O25 W7 117.2(4) . .
W7 O27 W8 117.5(4) . .
W7 O28 Fe1 143.3(5) . .
W8 O30 W9 146.8(5) . .
W8 O31 Fe2 134.4(5) . .
W9 O33 Fe2 137.4(5) . .
O5W Eu1 O12W 142.3(6) . .
O5W Eu1 O9W 127.6(6) . .
O12W Eu1 O9W 73.8(6) . .
O5W Eu1 O8W 77.5(6) . .
O12W Eu1 O8W 134.6(5) . .
O9W Eu1 O8W 99.3(6) . .
O5W Eu1 O6W 81.2(6) . .
O12W Eu1 O6W 76.7(5) . .
O9W Eu1 O6W 73.0(5) . .
O8W Eu1 O6W 145.5(5) . .
O5W Eu1 O11W 98.4(7) . .
O12W Eu1 O11W 76.9(7) . .
O9W Eu1 O11W 132.2(7) . .
O8W Eu1 O11W 76.0(7) . .
O6W Eu1 O11W 134.3(5) . .
O5W Eu1 O7W 63.0(7) . .
O12W Eu1 O7W 140.7(7) . .
O9W Eu1 O7W 68.6(7) . .
O8W Eu1 O7W 64.4(7) . .
O6W Eu1 O7W 81.8(6) . .
O11W Eu1 O7W 138.7(7) . .
O5W Eu1 O19 69.1(5) . .
O12W Eu1 O19 74.6(5) . .
O9W Eu1 O19 135.1(4) . .
O8W Eu1 O19 125.6(5) . .
O6W Eu1 O19 69.2(3) . .
O11W Eu1 O19 68.2(5) . .
O7W Eu1 O19 126.9(6) . .
O5W Eu1 O10W 139.1(7) . .
O12W Eu1 O10W 74.5(7) . .
O9W Eu1 O10W 67.9(7) . .
O8W Eu1 O10W 61.9(7) . .
O6W Eu1 O10W 136.4(7) . .
O11W Eu1 O10W 68.2(8) . .
O7W Eu1 O10W 100.9(8) . .
O19 Eu1 O10W 130.9(6) . .
O33 Fe2 O31 86.7(4) . .
O33 Fe2 O4 96.5(4) . 2_666
O31 Fe2 O4 96.4(3) . 2_666
O33 Fe2 O34 91.5(4) . .
O31 Fe2 O34 90.6(4) . .
O4 Fe2 O34 169.7(4) 2_666 .
O33 Fe2 O3W 93.4(4) . .
O31 Fe2 O3W 176.7(4) . .
O4 Fe2 O3W 86.9(4) 2_666 .
O34 Fe2 O3W 86.1(4) . .
O33 Fe2 O4W 175.3(4) . .
O31 Fe2 O4W 90.1(4) . .
O4 Fe2 O4W 87.2(4) 2_666 .
O34 Fe2 O4W 85.1(4) . .
O3W Fe2 O4W 89.6(5) . .
C1 O34 Fe2 143.7(16) . .
C1 O35 H35A 109.5 . .
C3 O36 H36A 109.5 . .
C2 N1 H1A 120.0 . .
C2 N1 H1B 120.0 . .
H1A N1 H1B 120.0 . .
O34 C1 O35 125(3) . .
O34 C1 C2 122(2) . .
O35 C1 C2 113(2) . .
O34 C1 O24W 90.9(19) . 2_666
O35 C1 O24W 77.4(18) . 2_666
C2 C1 O24W 108(2) . 2_666
C3 C2 N1 128(3) . .
C3 C2 C1 112(2) . .
N1 C2 C1 105(2) . .
C3 C2 H2A 102.5 . .
N1 C2 H2A 102.5 . .
C1 C2 H2A 102.5 . .
O36 C3 C2 101(2) . .
O36 C3 C4 99(2) . .
C2 C3 C4 110(3) . .
O36 C3 H3A 114.9 . .
C2 C3 H3A 114.9 . .
C4 C3 H3A 114.9 . .
C3 C4 H4A 109.5 . .
C3 C4 H4D 109.5 . .
H4A C4 H4D 109.5 . .
C3 C4 H4B 109.5 . .
H4A C4 H4B 109.5 . .
H4D C4 H4B 109.5 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Sb1 O2 1.991(8) .
Sb1 O14 2.001(8) .
Sb1 O23 2.003(8) .
W1 O4 1.768(8) .
W1 O1 1.775(9) .
W1 O3 1.791(9) .
W1 O6' 1.96(6) .
W1 O5 2.038(16) .
W1 O6 2.063(14) .
W1 O5' 2.08(6) .
W1 O2 2.231(8) .
W2 O7 1.712(9) .
W2 O10' 1.73(5) .
W2 O6' 1.79(6) .
W2 O8 1.876(8) .
W2 O6 1.892(14) .
W2 O9 1.956(8) .
W2 O10 2.000(12) .
W2 O2 2.349(8) .
W3 O11 1.729(9) .
W3 O5' 1.84(6) .
W3 O10 1.885(14) .
W3 O5 1.887(16) .
W3 O13 1.889(8) .
W3 O12 1.972(8) .
W3 O10' 2.04(6) .
W3 O2 2.350(8) .
W4 O15 1.714(9) .
W4 O17 1.828(8) .
W4 O16 1.936(8) .
W4 O18 1.950(8) .
W4 O13 1.971(8) .
W4 O14 2.289(8) .
W5 O19 1.747(8) .
W5 O12 1.863(8) .
W5 O21 1.885(9) .
W5 O20 1.914(8) .
W5 O18 1.937(8) .
W5 O14 2.251(8) .
W6 O22 1.711(8) .
W6 O9 1.894(8) .
W6 O25 1.904(9) .
W6 O24 1.918(8) .
W6 O21 1.922(9) .
W6 O23 2.310(8) .
W7 O26 1.723(9) .
W7 O28 1.814(8) .
W7 O27 1.913(8) .
W7 O8 1.963(8) .
W7 O25 1.979(8) .
W7 O23 2.304(8) .
W8 O29 1.747(8) .
W8 O31 1.818(9) .
W8 O30 1.894(9) .
W8 O27 1.971(8) .
W8 O24 1.994(8) .
W8 O23 2.233(8) .
W9 O32 1.732(9) .
W9 O33 1.838(8) .
W9 O16 1.933(8) .
W9 O30 1.968(9) .
W9 O20 1.975(8) .
W9 O14 2.298(8) .
Fe1 O17 1.942(8) 2_666
Fe1 O28 1.943(9) .
Fe1 O3 1.974(9) .
Fe1 O1 2.011(9) 2_666
Fe1 O2W 2.061(9) .
Fe1 O1W 2.062(9) .
O5W Eu1 2.410(18) .
O6W Eu1 2.451(11) .
O7W Eu1 2.46(2) .
O8W Eu1 2.443(18) .
O9W Eu1 2.437(14) .
O10W Eu1 2.51(2) .
O11W Eu1 2.455(18) .
O12W Eu1 2.426(14) .
O23W O22W 1.66(5) 2_666
O22W O23W 1.66(5) 2_666
O24W C1 1.89(4) 2_666
O1 Fe1 2.011(9) 2_666
O4 Fe2 1.985(8) 2_666
O17 Fe1 1.942(8) 2_666
O19 Eu1 2.470(9) .
O31 Fe2 1.979(9) .
O33 Fe2 1.933(9) .
Fe2 O4 1.985(8) 2_666
Fe2 O34 2.033(9) .
Fe2 O3W 2.054(10) .
Fe2 O4W 2.069(10) .
O34 C1 1.11(3) .
O35 C1 1.32(3) .
O35 H35A 0.8200 .
O36 C3 1.40(3) .
O36 H36A 0.8200 .
N1 C2 1.468(10) .
N1 H1A 0.8600 .
N1 H1B 0.8600 .
C1 C2 1.54(3) .
C1 O24W 1.89(4) 2_666
C2 C3 1.44(3) .
C2 H2A 0.9800 .
C3 C4 1.60(4) .
C3 H3A 0.9800 .
C4 H4A 0.9600 .
C4 H4D 0.9600 .
C4 H4B 0.9600 .
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
O35 H35A O4W 0.82 2.37 3.08(2) 144.4 .
O35 H35A O25W 0.82 2.47 3.12(2) 136.6 2_656
O36 H36A O24W 0.82 1.80 2.58(3) 158.4 2_666
O36 H36A O12W 0.82 2.34 2.81(2) 117.3 2_655
N1 H1A O22W 0.86 2.15 2.97(5) 160.2 2_655
N1 H1B O30 0.86 2.35 3.12(2) 150.2 .
N1 H1B O29 0.86 2.39 3.06(2) 135.4 .
